## Doping screening of polarization fields in nitride heterostructures

Aldo Di Carlo, Fabio Della Sala, Paolo Lugli, Vincenzo Fiorentini, and Fabio Bernardini

Citation: Appl. Phys. Lett. 76, 3950 (2000); doi: 10.1063/1.126831 View online: http://dx.doi.org/10.1063/1.126831

View Table of Contents: http://apl.aip.org/resource/1/APPLAB/v76/i26

Published by the American Institute of Physics.

### Related Articles

Thermal carrier emission and nonradiative recombinations in nonpolar (Al,Ga)N/GaN quantum wells grown on bulk GaN

J. Appl. Phys. 111, 033517 (2012)

Surface depletion mediated control of inter-sub-band absorption in GaAs/AlAs semiconductor quantum well systems

Appl. Phys. Lett. 100, 051110 (2012)

High-Q optomechanical GaAs nanomembranes

Appl. Phys. Lett. 99, 243102 (2011)

Mg-induced terahertz transparency of indium nitride films

Appl. Phys. Lett. 99, 232117 (2011)

Effect of metal-precursor gas ratios on AlInN/GaN structures for high efficiency ultraviolet photodiodes

J. Appl. Phys. 110, 103523 (2011)

### Additional information on Appl. Phys. Lett.

Journal Homepage: http://apl.aip.org/

Journal Information: http://apl.aip.org/about/about_the_journal

Top downloads: http://apl.aip.org/features/most_downloaded

Information for Authors: http://apl.aip.org/authors

**Doping screening of polarization fields in nitride heterostructures**

Aldo Di Carlo,a)Fabio Della Sala, and Paolo Lugli

*INFM and Dipartimento di Ingegneria Elettronica, Universita` di Roma ‘‘Tor Vergata,’’ I-00133 Rome,*
*Italy*

Vincenzo Fiorentini and Fabio Bernardini

*INFM and Dipartimento di Fisica, Universita` di Cagliari, I-09100 Cagliari, Italy*

共Received 15 February 2000; accepted for publication 9 May 2000兲

Using self-consistent tight-binding calculations, we show that modulation doping can be used to
screen macroscopic polarization fields in nitride quantum wells. The blue-shift of
photoluminescence peak as well as the reduction of radiative recombination lifetime at increasing
doping density is explained and correlated to polarization-field screening. The field-induced
ionization of the dopants and its relation with alloy composition in the heterostructure barriers is
*also analyzed. © 2000 American Institute of Physics.*关S0003-6951共00兲05026-9兴

Laser structures based on III–V nitride multiquantum wells 共MQWs兲 have been shown to benefit from doping of the active region.1However, several puzzles remain concern-ing the mechanisms involved. Experimentally, it has been established for both GaN/InGaN2–9 and AlGaN/GaN10–12 heterostructures that doping of the active region produces共i兲 a blue-shift of the photoluminescence 共PL兲 peak, 共ii兲 an en-hancement of the emission intensity, 共iii兲 a reduction of the laser threshold current, 共iv兲 a reduction of the carrier radia-tive recombination lifetime, and共v兲 a reduction of the Stokes shift between PL peak and the photoluminescence excitation

共PLE兲 spectra. Based on phenomenological arguments, it has

been suggested that the observed phenomena is due to 共a兲 doping-enhanced growth quality of the active region,3,4,8,11,13

共b兲 doping screening of polarization fields,3,5,6,9_{or}_{共c兲 }
screen-ing of potential fluctuations.4–6,8

Despite its relevance to laser design, the doping effect
has been only marginally touched upon theoretically.9,14 In
this letter we apply the self-consistent procedure outlined in
Refs. 14–16 to AlGaN/GaN and GaN/InGaN MQW systems,
investigating how piezoelectric and spontaneous14,17–19
*po-larization fields can be screened via n- and p-type doping.*
Further, we consider the screening interplay of extrinsic and
injected carriers, experimentally investigated in Ref. 6.

We solve the Schro¨dinger equation in the
nearest-neighbor *s p*3*d*5*s** tight-binding 共TB兲 basis,20
self-consistently coupled with a one-dimensional 共1D兲 Poisson
equation accounting for polarization, doping, and free
carriers.14–16The macroscopic polarization in the alloys are
*obtained by Vegard interpolation of ab initio values*17for the
binary compounds. This procedure describes the interplay of
polarization and dielectric, free-carrier, and doping screening
in a fully self-consistent and nonperturbative way, with band
*structure accuracies typical of ab initio methods.*20 Optical
properties are obtained via the Graf–Vogl theory21 without
introducing additional fitting parameters. The method has
been previously employed to describe wide-gap MQW and
interface systems.14,15,19,22

We performed calculations at room temperature for

Al0.15Ga0.85N/GaN and In0.2Ga0.8N/GaN MQWs, with 100 Å barriers and 40 Å wells, pseudomophically grown on a GaN substrate. We considered purposely modulation-doped

共doped barrier兲 structures, assuming a 1017_{cm}⫺3 _{residual}
doping in the wells. The extrinsic levels are chosen among a
20 meV bound donor, and shallow 共20 meV兲 or deep 共250
meV兲 acceptors, the ‘‘deep’’ level representing typical

*p-dopants in GaN.*23

The results for the AlGaN/GaN MQWs are shown in
Fig. 1. The optical gap 关the separation between the first
quantized conduction共C1兲 and valence 共V1兲 levels兴 and the
C1–V1 oscillator strength共proportional to the C1–V1
radia-tive transition probability兲 are plotted respectively in Figs.
1共a兲 and 1共b兲 as a function of the doping density, for several
*values of an externally injected free carrier density (n2D*).
Inclusion of the latter allows us to mimic lasing under
elec-trical or optical pumping.

a兲_{Electronic mail: [email protected]}

FIG. 1. Ground-level-emission transition energy共a兲 and oscillator strength
共b兲 in Al0.15Ga0.85*N/GaN MQWs, as a function of p or n doping densities, at*
different values of free-charge injection.

APPLIED PHYSICS LETTERS VOLUME 76, NUMBER 26 26 JUNE 2000

3950

0003-6951/2000/76(26)/3950/3/$17.00 © 2000 American Institute of Physics

*At zero injection (n2D*⫽0), the extrinsic carriers from
ionized dopants partially screen the macroscopic polarization
*field. For both n- and shallow p-doping, the fundamental*
transition energy blue-shifts by as much as 150 meV when
the doping density is increased from 1017_{to 3}_{⫻10}19_{cm}⫺3_{兲.}
Deep 共i.e., the actual兲 acceptors are much less efficient in
screening the polarization and cause a blue-shift of only 80
meV. Indeed, larger dopant binding energy implies fewer
ionized centers, hence fewer free carriers in the well. Upon
free-carrier injection, the doping-induced blue-shift is
re-duced. This is expected since screening is already activated
by the injected free charge itself共notably at high injection兲.
The radiative probability of the C1–V1 transition 关Fig.
1共b兲兴 is related to the laser threshold current. In the absence
of carrier injection, the transition probability increases by an
order of magnitude in going from low to high doping
densi-ties. In fact, doping screening of the field increases the
over-lap between confined conduction and valence states,
enhanc-ing the radiative transition probability. We found that the
*increase in transition probability is lower for shallow p *
*dop-ing than for n dopdop-ing. This result depends on the different*
density of states and band offsets for electron and holes.

For laser operation, however, the case with injected
car-riers is more relevant. As for the transition energy, the higher
the injected density, the smaller the doping-induced shift: at
high injection, the polarization field is already screened even
for low doping. However, for typical laser-operation
densi-ties, a moderately high doping does increase the transition
probability. For 1019cm⫺3doping, one obtains the the same
*recombination probability at injection n2D*⫽5⫻1012cm⫺2as
*at n2D*⫽1013cm⫺2with no doping. Since the recombination
probability is inversely proportional to the spontaneous
combination lifetime, the laser threshold current will be
re-duced by proper doping design.

The doping dependence of transition energies and prob-ability in GaN/InGaN MQWs is shown in Figs. 2共a兲 and 2共b兲, respectively. The overall effect of doping is stronger

than in the AlGaN/GaN case, the blue-shift amounting to
*280 meV for n doping and for deep-level p doping, and up to*
*325 meV for shallow-level p doping. The higher efficiency*
of doping screening in GaN/InGaN wells is due to
polariza-tion field being larger than in AlGaN/GaN ones 共the
polar-ization charge is 0.03 C/m2 at GaN/In0.2Ga0.8N interfaces,
compared to 0.013 C/m2 at Al0.15Ga0.85N/GaN ones兲. The
field-induced ionization 共FII兲 of the dopant 共already pointed
out in Ref. 24兲 is consequently larger in the GaN/InGaN than
the in AlGaN/GaN structure. The FII effect is also
*respon-sible for the comparable effectiveness of the deep p and*

*n-type doping. Under high injection condition, the same*

trends are observed as in the AlGaN/GaN case.

The degree of field ionization of the dopants in the
bar-riers depends on the barrier material, via the alloy
composi-tion dependence of polarizacomposi-tion fields. Hence, the screening
efficiency should depend on composition. Indeed, consider
Fig. 3, displaying the C1–V1 transition blue-shift obtained
by raising the doping density from 1017to 3⫻1019cm⫺3, as
a function of Al concentration in the AlGaN barrier, and
*considering both n and deep p doping. The increased Al*
content enhances the electric field in the structure, hence the
ionized dopant density: consequently the blue-shift is larger
at large Al concentrations. Again, the deeper level screens
less efficiently.

Neglect of polarization yields, as expected, a shift which
is negligible on the relevant energy scale. This does not
*nec-essarily imply that the density of ionized impurities is *
re-duced when polarization fields are neglected. While this is
*the case for p doping because of the acceptor depth,*24 it is
*not for n doping, where the percentage of ionized dopants*
with and without polarization fields are comparable. As Fig.
4 shows, the key effect of the field is to ionize the impurities

*asymmetrically. The ionized* 共positive兲 centers and the

elec-trons transferred into the well form a dipole which screens the field. If the field is zero, the ionization will be symmetric with respect to the quantum well, and no dipole will result.

In conclusion, we have shown that doping induces a blue-shift of the optical transition, larger for low injected carrier density. Doping increases the transition probability at the optical gap. This explains the experimental findings of lower laser threshold current, reduced radiative lifetime, and increased emission intensity in doped MQWs. Because of field ionization of the dopants, the doping screening effi-ciency depends on heterostructure composition. All free-FIG. 2. As in Fig. 1, for GaN/In0.2Ga0.8N MQWs.

*FIG. 3. Shift of the C1–V1 transition vs x in Alx*Ga1*⫺x*N/GaN MQWs,

calculated as the difference of the C1–V1 transitions for doping levels of
3⫻1019_{and 10}17_{cm}⫺3_{.}

3951

Appl. Phys. Lett., Vol. 76, No. 26, 26 June 2000 Di Carloet al.

charge related values 共such as blue-shifts, PL intensity, Stokes-shifts, etc.兲 will thus depend both on doping and ma-terial composition. We conclude that doping is an additional degree of freedom to tune nitride lasers for efficiency.

Work supported in part by MURST, ‘‘Ultrafast Quantum Electronics’’ and ‘‘CLERMONT’’ UE Networks, and INFM through a PAISS Project.

1_{S. Nakamura, M. Senoh, A. Nagahama, N. Iwasa, T. Yamada, T. }

**Mat-sushita, and H. Kiyoku, Appl. Phys. Lett. 70, 2753**共1997兲; S. Nakamura,
M. Senoh, A. Nagahama, N. Iwasa, T. Yamada, T. Matsushita, H. Kiyoku,
* Y. Sugimoto, T. Kozaki, H. Umemoto, M. Sano, and K. Chocho, ibid., 72,*
2014

**共1998兲; 73, 832 共1998兲.**

2_{P. A. Grudowski, C. J. Eiting, J. Park, B. S. Shelton, D. J. H. Lambert, and}

**R. D. Dupuis, Appl. Phys. Lett. 71, 1537**共1997兲; S. Bidnyk, T. J. Schmidt,
Y. H. Cho, G. H. Gainer, J. J. Song, S. Keller, U. K. Mishra, and S. P.
* DenBaars, ibid., 72, 1623*共1998兲.

3_{M. S. Minsky, S. Chichibu, S. B. Fleisher, A. C. Abare, J. E. Bowers, E.}

L. Hu, S. Keller, U. K. Mishra, and S. P. DenBaars, Jpn. J. Appl. Phys.,
**Part 2 37, L1362**共1998兲.

4_{Y.-H. Cho, J. J. Song, S. Keller, M. S. Minsky, E. Hu, U. K. Mishra, and}

**S. P. DenBaars, Appl. Phys. Lett. 73, 1128**共1998兲.

5_{T. Deguchi, A. Shikanai, K. Torii, T. Sota, S. Chichibu, and S. Nakamura,}

**Appl. Phys. Lett. 72, 3329**共1998兲; S. Chichibu, D. A. Cohen, M. P. Mack,
A. C. Abare, P. Kozodoy, M. Minsky, S. Fleisher, S. Keller, J. E. Bowers,

* U. K. Mishra, l. A. Coldren, D. R. Clarke, and S. P. DenBaars, ibid., 73,*
496共1998兲.

6_{J. Dalfors, J. P. Bergman, P. O. Holtz, B. E. Sernelius, B. Monemar, H.}

**Amano, and I. Aksaki, Appl. Phys. Lett. 74, 3299**共1999兲.

7

K. Uchida, T. Tang, S. Goto, T. Mishima, A. Niw, and J. Gotoh, Appl.
**Phys. Lett. 74, 1153**共1999兲.

8_{Y.-H. Cho, F. Fedler, R. J. Hauenstein, G. H. Park, J. J. Song, S. Keller,}

**U. K. Mishra, and S. P. DenBaars, J. Appl. Phys. 85, 3006**共1999兲.

9_{H. Jiang, M. Minsky, S. Keller, E. Hu, J. Singh, and S. P. DenBaars, IEEE}

**J. Quantum Electron. 35, 1483**共1999兲.

10

A. Salvador, G. Liu, W. Ki, O. Aktas, A. Botchkarev, and H. Morkoc,
**Appl. Phys. Lett. 67, 3322**共1995兲.

11_{K. C. Zeng, J. Y. Lin, H. X. Jiang, A. Salvador, G. Popovici, H. Tang, W.}

**Kim, and H. Morkoc, Appl. Phys. Lett. 71, 1368**共1997兲.

12_{H. Hirajama and Y. Aoyagi, MRS Internet J. Nitride Semicond. Res. 4S1,}

G3.74共1999兲.

13

S. I. Molina, A. M. Sanchez, F. J. Pacheco, R. Garcia, M. A.
**Sanchez-Garcia, F. J. Sanchez, and E. Calleja, Appl. Phys. Lett. 74, 3362**共1999兲.

14_{V. Fiorentini, F. Bernardini, F. Della Sala, A. Di Carlo, and P. Lugli,}

**Phys. Rev. B 60, 8849**共1999兲.

15_{F. Della Sala, A. Di Carlo, P. Lugli, F. Bernardini, V. Fiorentini, R.}

**Scholtz, and J. M. Jancu, Appl. Phys. Lett. 74, 2002**共1999兲.

16

A. Di Carlo, S. Pescetelli, M. Paciotti, P. Lugli, and M. Graf, Solid State
**Commun. 98, 803**共1996兲; A. Di Carlo, Phys. Status Solidi B , 703 共2000兲.

17_{F. Bernardini, V. Fiorentini, and D. Vanderbilt, Phys. Rev. B 56, R10024}* 共1997兲; F. Bernardini and V. Fiorentini, ibid., 57, R9427 共1998兲.*
18

_{M. Leroux, N. Grandjean, M. Laugt, J. Massies, B. Gil, P. Lefebvre, and}

**P. Bigenwald, Phys. Rev. B 58, R13371**共1998兲.

19_{R. Cingolani, A. Botchkarev, H. Tang, H. Morkoc, G. P. Traetta, G. Colı`,}

**M. Lomascolo, A. Di Carlo, F. Della Sala, and P. Lugli, Phys. Rev. B 61,**
2711共2000兲.

20** _{J-M. Jancu, R. Scholz, F. Beltram, and F. Bassani, Phys. Rev. B 57, 6493}**
共1998兲.

21_{M. Graf and P. Vogl, Phys. Rev. B 51, 4940}_{共1995兲.}
22

G. Traetta, R. Cingolani, A. Di Carlo, F. Della Sala, and P. Lugli, Appl.
**Phys. Lett. 76, 1042**共2000兲; A. Bonfiglio, M. Lomascolo, G. Traetta, R.
Cingolani, A. Di Carlo, F. Della Sala, P. Lugli, A. Botchkarev, and H.
**Morkoc, J. Appl. Phys. 87, 2289**共2000兲; A. Rizzi, R. Lantier, F. Monti, H.
**Lu¨th, F. Della Sala, A. Di Carlo, and P. Lugli, J. Vac. Sci. Technol. B 17,**
1674共1999兲.

23

*J. Neugebauer and C. van de Walle, in Advances in Solid State Physics*

共Vieweg, Braunschweig, 1996兲, Vol. 35, p. 25. 24

P. Kozodoy, Y. P. Smorchkova, M. Hansen, H. Xing, S. P. DenBaars, U. K. Mishra, A. W. Saxler, R. Perrin, and W. C. Mitchell, Appl. Phys. Lett.

**75, 2444**共1999兲.
FIG. 4. Ionized dopant density 共dashed lines兲 and electron density 共solid

line*兲 in a n-doped (3⫻10*19_{cm}⫺3_{) Al}

0.15Ga0.85N/GaN MQW.

3952 Appl. Phys. Lett., Vol. 76, No. 26, 26 June 2000 Di Carloet al.